Porous silicon/Ni composites of high coercivity due to magnetic field-assisted etching
© Granitzer et al.; licensee Springer. 2012
Received: 30 April 2012
Accepted: 26 June 2012
Published: 11 July 2012
Ferromagnetic nanostructures have been electrodeposited within the pores of porous silicon templates with average pore diameters between 25 and 60 nm. In this diameter regime, the pore formation in general is accompanied by dendritic growth resulting in rough pore walls, which involves metal deposits also offering a branched structure. These side branches influence the magnetic properties of the composite system not only due to modified and peculiar stray fields but also because of a reduced interpore spacing by the approaching of adjacent side pores. To improve the morphology of the porous silicon structures, a magnetic field up to 8 T has been applied during the formation process. The magnetic field etching results in smaller pore diameters with less dendritic side pores. Deposition of a ferromagnetic metal within these templates leads to less branched nanostructures and, thus, to an enhancement of the coercivity of the system and also to a significantly increased magnetic anisotropy. So magnetic field-assisted etching is an appropriate tool to improve the structure of the template concerning the decrease of the dendritic pore growth and to advance the magnetic properties of the composite material.
KeywordsMagnetic field-assisted anodization Porous silicon Magnetic nanostructures 68.65.-k 75.75.-c 81.07.-b
In recent years, the demand on nanostructured materials increased enormously not only because of the miniaturization of devices but also because of the appearance of modified physical properties of nanosized objects compared to their bulk material. Nanostructures can be achieved by a top-down or bottom-up approach, whereas nanostructuring by self-organization is an emerging topic due to less costs, less time consumption and mostly a simple fabrication procedure.
Porous silicon can be formed with various morphologies  exhibiting structures between a few nanometers and several tens of micrometers, and in its different natures, it is a versatile material for a broad range of applications in optics , acoustics  and sensor technology , and in biomedicine, it is promising due to its biodegradability and biocompatibility . The possibility of achieving straight pores renders porous silicon a good template material for the deposition of various metals , whereas the case of merging ferromagnetic nanostructures with a semiconducting substrate results in a hybrid material, which offers the electronic properties of silicon and the nanomagnetic behavior of the precipitates. The deposition of the metals within the pores can be achieved electroless, electrochemically or by vapor transport methods such as atomic layer deposition or a form of chemical vapor deposition.
The fabrication of specimens with specific magnetic properties can be reached due to the possibility of modifying the geometry and the packing density of the precipitated metal nanostructures as well as of varying the morphology of the template . Considering the deposition of metal wires within the pores, a magnetic anisotropy between the two magnetization directions, with an applied field perpendicular (easy axis) and parallel (hard axis) to the surface, can be observed. The metal wires interact dipolarly not only within the pores but also between adjacent pores, depending on the pore distance. To enhance this anisotropy, the magnetostatic interactions between adjacent pores have to be decreased. Thus, the application of a magnetic field during the etching procedure has been employed to achieve smoother pore walls, leading also to smoother metal deposits, which results in a bigger effective distance between adjacent metal structures.
Both types of templates, conventionally etched and magnetic field-etched ones, have been filled with Ni electrochemically. As electrolyte, a solution consisting of NiCl2, NiSO4 and H3BO3 has been employed. The galvanic deposition has been performed in a pulsed way . In choosing a current density of 12 mA/cm2 and a pulse frequency of 0.2 Hz, Ni-nanowires of a few micrometer in length were successfully embedded into the pores. The deposited Ni structures exhibit in all cases a wire-like structure with an aspect ratio up to 100. The precipitated Ni-wires within conventionally etched porous silicon offer roughness with a branched structure. In using the magnetic field-etched porous silicon as a template, the precipitated Ni-wires are smoother, and the mean distance between neighboring pores is increased up to 50 nm.
To investigate the prepared nanocomposite systems structurally, mainly SEM and EDX spectroscopy is used. Magnetic characterization has been carried out by SQUID magnetometry and a vibrating sample magnetometer.
Results and discussion
Considering the dissolution process of silicon, holes diffusing to the silicon/electrolyte interface attack the silicon atoms, but the motion of the holes cannot be controlled easily. The application of a magnetic field perpendicular to the sample surface during the anodization process controls this motion of the holes moving from the bulk silicon to the pore-tip region. In this case, the holes only reach the pore tips and do not diffuse any further to the pore walls. Holes moving in the growth direction of the pores contribute to the formation process, whereas holes with a direction that deviates from the growth direction feel the Lorentz force, which is induced by the applied magnetic field and do not contribute to the dissolution of the silicon. This experimental arrangement results in smaller pore diameters and smoother pore walls compared to conventional etching with adequate electrochemical parameters .
Electrodeposition of Ni within these less dendritic templates results also in smoother Ni-wires with less side pores. Thus, on the one hand, the geometry of the wires with less dendrites and, on the other hand, the resulting bigger distance between adjacent pores influence the magnetic properties of the composite system. Comparing the samples with deposited Ni-wires, in which the porous silicon was prepared by either conventional etching or by magnetic field-assisted etching, a significant modification of the magnetic properties was observed.
Magnetization data measured at T = 4 K and T = 250 K
Coercivity (Oe) magnetic field perpendicular to surface
Coercivity (Oe) magnetic field parallel to surface
Remanence M/MS(emu) magnetic field perpendicular to surface
Remanence M/MS(emu) magnetic field parallel to surface
T = 4 K (conv.)
T = 100 K (conv.)
T = 250 K (conv.)
T = 4 K (mag.)
T = 100 K (mag.)
T = 250 K (mag.)
In the presented work, the modification of the magnetic properties of porous silicon/Ni nanocomposites caused by magnetic field-assisted pore formation is discussed. The high-aspect-ratio pores fabricated by anodization with an applied magnetic field offer a pore diameter smaller than 30 nm and a remarkable decreased growth of side pores. The deposition of Ni structures within these pores results in a more-than-doubled coercivity (increase from 270 to 650 Oe) and a doubled remanence (from 0.42 to 0.85 emu) of the nanocomposite compared to samples etched without magnetic field, whereas the aspect ratio of the deposited wires is comparable. The enhanced values can be attributed to the reduced magnetostatic interactions between Ni-wires deposited within neighboring pores, mainly caused by smoothened walls of the wires and an enhanced distance between the pores.
This work is supported by the Austrian Science Fund FWF under project P21155.
- Lehmann V: Electrochemistry of Silicon: Instrumentation, Science, Materials and Applications. Wiley-VCH, Weinheim; 2002.View ArticleGoogle Scholar
- Canham LT, Stewart MP, Buriak JM, Reeves CL, Anderson M, Squire EK, Allock P, Snow PA: Derivatized porous silicon mirrors: implantable optical components with slow resorbability. Phys Status Solidi A Appl Res 2000, 182: 521. 10.1002/1521-396X(200011)182:1<521::AID-PSSA521>3.0.CO;2-7View ArticleGoogle Scholar
- Koshida N, Ohta T, Gelloz B, Kojima A: Ballistic electron emission from quantum-sized nanosilicon diode and its applications. Curr Opin Solid State Mater Sci 2011, 15: 183. 10.1016/j.cossms.2011.04.003View ArticleGoogle Scholar
- Boarino L, Baratto C, Geobaldo F, Amato G, Comini E, Rossi AM, Faglia G, Lerondel G, Sberveglieri G: NO2 monitoring at room temperature by a porous silicon gas sensor. Mater Sci Eng B 2000, 69–70: 210.View ArticleGoogle Scholar
- Canham LT: Bioactive silicon structure fabrication through nanoetching techniques. Adv Mater 1995, 7: 1033. 10.1002/adma.19950071215View ArticleGoogle Scholar
- Ogata YH, Kobayashi K, Motoyama M: Electrochemical metal deposition on silicon. Curr Opin Solid State Mater Sci 2006, 10: 163. 10.1016/j.cossms.2007.02.001View ArticleGoogle Scholar
- Rumpf K, Granitzer P, Albu M, Pölt P: Electrochemically fabricated silicon/metal hybrid nanosystem with tailored magnetic properties. Electrochem Solid State Lett 2010, 13: K15. 10.1149/1.3269188View ArticleGoogle Scholar
- Granitzer P, Rumpf K, Roca AG, Morales MP, Poelt P, Albu M: Investigation of a mesoporous silicon based ferromagnetic nanocomposite. NRL 2010, 5: 374.View ArticleGoogle Scholar
- Rumpf K, Granitzer P, Pölt P: Influence of the electrochemical process parameters on the magnetic behaviour of a silicon/metal nanocomposite. ECS Trans 2010, 25: 157.View ArticleGoogle Scholar
- Hippo D, Nakamine Y, Urakawa K, Tsuchiya Y, Mizuta H, Koshida N, Oda S: Formation mechanism of 100-nm-scale periodic structures in silicon using magnetic-field-assisted anodization. Jpn J Appl Phys 2008, 47: 7398. 10.1143/JJAP.47.7398View ArticleGoogle Scholar
- Suess D, Breth L, Lee J, Fuger M, Vogler C, Bruckner F, Bergmair B, Huber T, Fidler J, Schrefl T: Calculation of coercivity of magnetic nanostructures at finite temperatures. Phys Rev B 2011, 84: 224421.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.